advertisement

Frequency Response of the Mechanochemically Synthesized AgI-Ag2O-B2O3 Superionic Glasses a Ankur Verma and K. Shahi Solid State Ionics Laboratory, Advanced Center for Materials Science a also in the Department of Physics Indian Institute of Technology Kanpur, India208016 Email: [email protected] Abstract: The synthesis of xAgI(1x)[Ag2O.B2O3] amorphous superionic conductors is done via mechanochemical synthesis route (for x = 0.5 and 0.7). Ionic conductivities of 31031cm1 for x = 0.5 sample and 51031cm1 for x = 0.7 sample at room temperature, are observed, which are higher than those of the melt quenched glassy samples. Impedance plots (Nyquist plots) are found to be depressed semicircles with a tail at low frequency end. The corresponding equivalent circuit is postulated and each circuit element is related to a physical process. The ac conductivity ( ) is analyzed in view of the universal dynamic response (UDR), ( ,T) = dc (T) + Ao(T) n (Bode Plots). A unique feature of the mechnochemically synthesized glasses is that their dc vs. 1/T behavior exhibit two distinct regions with different activation energies. The activation energy for dc conductivity (Edc) and that for ac conductivity (Eac) and the frequency exponent n are found to satisfy the UDRrelation, Eac= (1n)Edc in the lower temperature regime. In the high temperature region, however, this correlation could not be established due to lack of ac data over the available frequency domain. Keywords: Frequency response, mechanochemical synthesis, superionic glasses, ball milling. PACS Nos.: 66.30Dn, 72.80Ng Introduction Mechanochemical synthesis is a known and powerful technique to synthesize amorphous and nanocrystalline materials. However, only recently it has been used successfully to synthesize amorphous superionic conductors (aSICs). Being a room temperature process, it has obvious advantages over the other conventional techniques such as rapid quenching of the melt. The work deals with mechanochemical synthesis of aSIC and its electrical characterization by means of frequency response analysis via Nyquist and Bode plots to understand the nature of ion dynamics. After complete amorphization the residual acetone is vacuum evaporated. XRD was done to examine amorphization of the mechanochemically synthesized material. Electrical characterization was done using HP-4192A Impedance Analyzer in the temperature range 90425 K. Results and Discussion XRD results show the formation of glass due to mechanical milling. Fig. 1 shows the XRD pattern of the sample containing 50 mol% AgI with respect to the milling time. Experimental The starting materials were 99% pure silver iodide, silver oxide, and boron oxide supplied by Aldrich, USA. Appropriate amounts of the starting chemicals were taken in the agate pot with four balls each of diameter 18 mm and weighing 8 g. The ball is to material weight ratio was kept nearly 4 for optimum results. Milling was done in the FRITSCH Pulverisette 6 at 400 rpm in acetone medium for 3035 hours. The acetone level was monitored periodically and kept at a constant level. Samples were taken out at regular interval to examine the progress of amorphization. Nyquist plots of impedance are found to be depressed semicircles, which suggest the presence of a constant phase element (CPE) in parallel with a resistance like behavior of the system [1]. The constant phase element exponent or the depression parameter is calculated for these depressed semicircles and found to be 0.480.04. Amount of distortion in these depressed semicircles increases with increasing temperature (Fig. 2). The pure resistance (Rdc) is calculated form the Re(Z*)axis intercept of the depressed semicircle and used for the evaluation of dc conductivity (dc). Fig. 3 (a) shows the equivalent electrical circuit of the cell and in Fig. 3 (b), each circuit element is related to a physical process. The CPE-1 is due to the parallel plate capacitor formed by two silver electrodes, R is due to the electrolyte resistance and CPE-2 is due to the charge double layer formed at the electrode-electrolyte interface due to polarization at lower frequencies. (,T) = dc (T) + Ao(T)n … (1) Where 0< n 1 and dc is the frequency independent dc conductivity. dc is calculated from the plateau on the low frequency side of () isotherms (Fig. 4). The other two parameters of Eq. (1), i.e., A and n, are evaluated by allometric curve fitting [4]. At higher temperature when the glassy samples become more conducting, the electrical conductivity is observed to decrease at lower frequencies (<500 Hz), which can obviously be attributed to polarization effects. Thus the low frequency data (<500 Hz) have been neglected for the fitting purpose. 0.5 AgI 0.5[Ag2O.B2O3] MQ 30 hr Intensity (A.U.) conductivity in glasses is usually described by the so called universal dynamic response [2-3]. 24 hr 18 hr CPE-1 CPE-2 CPE-2 R 12 hr (a) 6 hr Electrolyte Electrodes 20 30 40 2 50 60 o Fig. 1: X-ray diffraction patterns of 0.5AgI-0.5(Ag2O-B2O3) samples mechanically milled for different durations at room temperature. Also shown is the result for melt quenched glass of the same composition. 0.7 AgI 0.3[Ag2O.B2O3] 20 (b) Figure 3: (a) Equivalent circuit diagram of the cell and (b) the physical processes occurring in the cell. * Im(Z ) k 15 10 5 155 K 161 K 166 K 0 0 5 10 15 20 * Re(Z ) k Figure 2: Nyquist plot of impedance for 70 mol % AgI samples at 155, 161 and 166 K. Fig. 4 shows the electrical conductivity as a function of frequency for 50 mol% AgI sample in the temperatures range 124248 K. The frequency dependence of electrical Fig. 5 compares the dc conductivities of the two samples, i.e., 50 and 70 mol% AgI, in the whole temperature range 150420 K. It is clearly noticed that there are two different conduction regimes, a low temperature region with a low activation energy (~0.15 eV) and a high temperature region with a higher activation energy Edc2 [5]. While both compositions have nearly same activation energy (~0.15 eV) within the experimental error ( 0.01 eV) in the low temperature regime, the 50 mol% AgI sample has higher activation energy (0.26 eV) than the 70 mol% AgI sample in the high temperature regime. The existence of two different activation regimes is a rather unusual behavior which may suggest the presence of two distinct bonding states of Ag+ ions in MM samples. It may be pointed out that MM SICs are reported to have two distinct crystallization temperatures [6], which is attributed 2 to the possible existence of two different environments for Ag+ ions. 10 0.5 AgI 0.5[Ag2O.B2O3] -3 248 K 212 10 -4 195 The other two parameters, i.e., A and n, of the UDR (Eq.1) are evaluated by the best fit method at different temperatures. Their variation as a function of inverse temperature is shown in Fig. 6. For both compositions A is found to be a thermally activated parameter with activation energies of Eac = 0.09 and 0.06 eV for 50 and 70 mol% AgI samples. However, the frequency exponent n, which is supposed to be a constant (0<n<1), is found to be a weakly temperature dependent parameter, decreasing with increasing temperature. The activation energies Eac and Edc and the exponent n are related as Ea c= (1n).Edc … … (2) -1 -1 ( cm ) 183 168 10 This condition is satisfied by the two amorphous samples in the low temperature regime if an average value of n is considered. On the basis of least square linear fit of the Figs. 4 and 5, the whole conductivity can be represented as a function of frequency and temperature as -5 151 142 10 -6 133 (,T) = o Exp(Edc/kT) + Ao Exp(Eac/kT)n(T) …(3) 124 10 2 10 3 10 4 10 5 10 6 /2 (Hz) Figure 4: Electrical conductivity as a function of frequency in the temperature range 124248 K for 50 mol % AgI sample (Bode plot). Exponential temperature dependence of dc and A (Eq.2) is widely accepted. But the temperature dependence of n is ambiguous. Weak temperature dependence of n was reported in the introductory papers by Jonscher [2-3]. Some others have reported n as an intrinsic material property and independent of temperature. The present study supports weak temperature dependence of n. T (K) -1 400 300 T (K) 150 200 200 10 180 160 140 120 0.55 0.5 AgI 0.5[Ag2OB2O3] 0.7 AgI 0.3[Ag2OB2O3] 0.5 AgI 0.5[Ag2O.B2O3] 0.50 -2 10 0.26 eV -1 -3 0.40 -1 10 Edc1= 0.15 eV -4 10 0.45 A ( cm ) -1 -1 ( cm ) -7 Edc2= 0.21 eV 0.16 eV Eac= 0.09 eV 0.35 -8 10 Frequency Exponent (n) 10 0.30 -5 10 2.5 3.0 3.5 4.0 4.5 5.0 5.5 6.0 6.5 -1 1000/T (K ) Figure 5: DC conductivities of 50 and 70 mole% AgI samples as a function of inverse temperature. Two distinct Arrhenius regions are evident. 0.25 5.5 6.0 6.5 7.0 7.5 8.0 -1 1000/T (K ) Figure 6: The variation of parameters A and n of UDR (Eq. 1) as a function of inverse of temperature for 50 mol % AgI sample. Clearly, n is decreasing with increasing temperature. 3 Conclusion Mechanically milled (MM) glasses are found to be different from the melt quenched (MQ) glasses in certain respects. For instance, the electrical conductivity of MM samples of 0.5AgI0.5[Ag2O.B2O3] is higher ( ~ 31031cm1 at 25C) and activation energy (Edc ~ 0.16 eV) lower than that for MQ glasses ( ~ 21031cm1, Ea ~ 0.36 eV at 25C). In addition to this, the dc(T) for MM samples has two distinct Arrhenius regions, while the MQ glasses just have one region. Also a relatively stronger temperature dependent n predicts some fundamental difference in the mechanism of conduction in MM glasses. The yAg2OzB2O3 glass is a poor ionic conductor ( < 10-5-1cm-1), so it is obvious that the mobile Ag+ ions are contributed by AgI only. Also the ratio of y:z is a defining parameter for the nature of glass. Hence, electrical measurements on xAgI.(1x)[yAg2O.zB2O3] system is required for different y:z ratios keeping x constant to understand the change in the nature of glass with varying y:z ratios. Also keeping y:z ratio constant and varying x one can find the fraction of Ag+ ions from the AgI contributing to the conductivity. References [1] J R Macdonald, “Impedance Spectroscopy: Emphasizing Solid Materials and Systems”, Wiley Interscience publications (1987). [2] A K Jonscher, Nature 267 (1977) 673. [3] K L Ngai, A K Jonscher and C T White, Nature 277 (1979) 185. [4] A Pradel, G Taillades, C Cramer and M Ribes, Solid State Ionics 105 (1998) 139. [5] S Kumar, K J Rao, Solid State Ionics 170 (2004) 191. [6] A Dalvi, PhD Thesis, IIT Kanpur, July 2003. [7] Ankur Verma, M.Tech. Thesis, IIT Kanpur, July 2004. 4